# Numerical Simulations of Stick Percolation: Application to the Study of Structured Magnetorheological Elastomers

Post on 09-Feb-2017

212 views

Embed Size (px)

TRANSCRIPT

Subscriber access provided by UNIVERSITY OF LEEDS

The Journal of Physical Chemistry C is published by the American Chemical Society.1155 Sixteenth Street N.W., Washington, DC 20036Published by American Chemical Society. Copyright American Chemical Society.However, no copyright claim is made to original U.S. Government works, or worksproduced by employees of any Commonwealth realm Crown government in the courseof their duties.

Article

Numerical Simulations of Stick Percolation: Application tothe Study of Structured Magnetorheological Elastomers

Jos Luis Mietta, Ricardo Martin Negri, and Pablo Ignacio TamboreneaJ. Phys. Chem. C, Just Accepted Manuscript DOI: 10.1021/jp504197w Publication Date (Web): 07 Aug 2014

Downloaded from http://pubs.acs.org on August 19, 2014

Just Accepted

Just Accepted manuscripts have been peer-reviewed and accepted for publication. They are postedonline prior to technical editing, formatting for publication and author proofing. The American ChemicalSociety provides Just Accepted as a free service to the research community to expedite thedissemination of scientific material as soon as possible after acceptance. Just Accepted manuscriptsappear in full in PDF format accompanied by an HTML abstract. Just Accepted manuscripts have beenfully peer reviewed, but should not be considered the official version of record. They are accessible to allreaders and citable by the Digital Object Identifier (DOI). Just Accepted is an optional service offeredto authors. Therefore, the Just Accepted Web site may not include all articles that will be publishedin the journal. After a manuscript is technically edited and formatted, it will be removed from the JustAccepted Web site and published as an ASAP article. Note that technical editing may introduce minorchanges to the manuscript text and/or graphics which could affect content, and all legal disclaimersand ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errorsor consequences arising from the use of information contained in these Just Accepted manuscripts.

Numerical Simulations of Stick Percolation:

Application to the Study of Structured

Magnetorheological Elastomers

J. L. Mietta, R. M. Negri, and P. I. Tamborenea,

Instituto de Qumica-Fsica de Materiales, Ambiente y Energa (INQUIMAE), Facultad de

Ciencias Exactas y Naturales, Universidad de Buenos Aires, Ciudad Universitaria, Pabelln II,

Ciudad de Buenos Aires, Argentina, and Departamento de Fsica and Instituto de Fsica de

Buenos Aires (IFIBA), Facultad de Ciencias Exactas y Naturales, Ciudad Universitaria, Pabelln

I, Ciudad de Buenos Aires, Universidad de Buenos Aires, Argentina

E-mail: pablot@df.uba.ar

To whom correspondence should be addressedINQUIMAEDepartamento de Fsica and IFIBA

1

Page 1 of 35

ACS Paragon Plus Environment

The Journal of Physical Chemistry

123456789101112131415161718192021222324252627282930313233343536373839404142434445464748495051525354555657585960

Abstract

In this article we explore how structural parameters of composites filled with one-dimensional,

electrically conducting elements (such as sticks, needles, chains, or rods) affect the percola-

tion properties of the system. To this end, we perform Monte Carlo simulations of asymmetric

two-dimensional stick systems with anisotropic alignments. We compute the percolation prob-

ability functions in the direction of preferential orientation of the percolating objects and in the

orthogonal direction, as functions of the experimental structural parameters. Among these, we

considered the average length of the sticks, the standard deviation of the length distribution,

and the standard deviation of the angular distribution. We developed a computer algorithm ca-

pable of reproducing and verifying known theoretical results for isotropic networks and which

allows us to go beyond and study anisotropic systems of experimental interest. Our research

shows that the total electrical anisotropy, considered as a direct consequence of the percolation

anisotropy, depends mainly on the standard deviation of the angular distribution and on the av-

erage length of the sticks. A conclusion of practical interest is that we find that there is a wide

and well-defined range of values for the mentioned parameters for which it is possible to ob-

tain reliable anisotropic percolation under relatively accessible experimental conditions when

considering composites formed by dispersions of sticks, oriented in elastomeric matrices.

Keywords: stick percolation, elastomers, nanowires.

1 Introduction and Experimental Motivation

Recently, a vigorous interest has arisen in percolating networks built out of nano- and micro-

dimensional objects (percolating objects), such as nanotubes and nanowires for various applica-

tions such as thin film transistors,1,2 flexible microelectronics,3 microelectromechanical systems

(MEMS),46 chemical sensors,7 and construction of transparent electrodes for optoelectronic and

photovoltaic devices.8,9 In particular, if these objects are used as fillers dispersed in an elastomeric

polymer and then oriented inside the organic matrix, there is an anisotropic internal structure to the

2

Page 2 of 35

ACS Paragon Plus Environment

The Journal of Physical Chemistry

123456789101112131415161718192021222324252627282930313233343536373839404142434445464748495051525354555657585960

material.10,11 This anisotropic structure can be obtained in practice following different methods,

like, for example, orienting the filler particles by means of an external field (electric or magnetic),

mechanically squeezing a composite material, etc. A particular case is given by magnetorheologi-

cal materials, whose mechanical properties can be modified by externally applied magnetic fields.

An important example of magnetorheological materials are composites formed by dispersing mag-

netic filler particles into an elastomer polymeric matrix and then orienting the particles. These

materials are referred to as magnetorheological elastomers (MRE). If, additionally, the filler par-

ticles are electrically conducting, the MRE may also be a conductor depending on the properties

of the filler and matrix materials, and on the conditions of synthesis. A simple procedure to ob-

tain MRE (in film or bulk form) consists of curing the filler-elastomer composite in the presence

of a uniform magnetic field, which induces agglomerations of the filler particles into chain-like

structures (needles) aligned in the direction of the magnetic field.4,6,1214

A desirable property in an electrically conducting MRE is its electrical anisotropy, i.e. its abil-

ity to conduct an electrical current preferentially in a special direction. Although we will not tackle

here the full problem of the relation between percolation and electrical conductivity, for our cur-

rent purposes it will suffice to use the fact that there will be total electrical anisotropy (TEA) in

the MRE, i.e. conduction in only a chosen direction, if there are percolating paths formed only in

that chosen direction. This direction is given by the preferred orientation of the needles, which

coincides with the direction of magnetic field applied during the curing of the material. For exam-

ple, TEA is a crucial property in devices like extended pressure mapping sensors,6,12 Zebra R-like

connectors for parallel flip-chip connections,4 and others. If the experimental variables are not

properly set during the fabrication of the MRE, a material devoid of anisotropy (or with very low

anisotropy) might be obtained,4,12,15 which would be unsuitable for these types of applications.

The microscopic structure of an MRE film filled with randomly distributed magnetic sticks can

be characterized by three parameters: the average length of the sticks, `, the standard deviation

of the length distribution, `, and the standard deviation of the angular distribution, (around a

chosen direction). As will be seen later, in the experimental samples these parameters correspond

3

Page 3 of 35

ACS Paragon Plus Environment

The Journal of Physical Chemistry

123456789101112131415161718192021222324252627282930313233343536373839404142434445464748495051525354555657585960

to a Gaussian distribution for the angle and a log-normal distribution for the length `. These

parameters can be set experimentally by changing the intensity of the magnetic field during the

curing, the exposure time to the magnetic field before starting the thermal curing, the viscosity of

the matrix, the amount of filler, the magnetic properties of the filler, etc. Two of us have performed

several experimental studies of these systems,4,6,12,13 and now we wish to understand how their

structural parameters affect the probability of obtaining systems with TEA. Nevertheless, it can be

expected that the results of our modeling will also apply to other composite materials with similar

internal structure.

In magnetorheological elastomers, micro- or nanoscopic objects (called alternatively chains,

needles, or sticks) are formed by magneto-piezo-electric manipulation under appropriate exper-

imental conditions at various stages of the synthesis process.4,6,12,15 These sticks formed by the

filler material can be considered as quasi-one-dimensional objects, so that the nanostructured MRE

as a whole can be analyzed in terms of networks of percolating sticks. Percolation can be studied

either in bulk (3D) or planar (2D) geometry. For our purposes (i.e. studying the TEA) both situa-

tions provide useful models, and we will therefore consider the latter, which allows us to explore

numerically larger systems. In rectangular or square MRE films, by definition there is a spanning

cluster if there is at least one connecting path between two opposing electrical contacts (located on

opposite edges of the film) formed by intersecting sticks. In order to relate electrical conduction to

percolation concepts, here we adopt the criterion that there is TEA if and only if there is a spanning

cluster in one direction and not in the other. Thus, we adopt here the well-known two-dimensional

model of percolating sticks, which is an example of a continuous percolation model1623 in order

to study the dependence of the TEA on the structural parameters , `, and `. We follow the

approach of studying the percolation probability functions in the direction of application of the

curing magnetic field and in the orthogonal direction, as functions of the experimental parameters

, `, and `. For this, we have developed a computer algorithm that is able to reproduce and

verify known theoretical results for isotropic networks and which allows us to go beyond and study

anisotropic systems of experimental interest.

4

Page 4 of 35

ACS Paragon Plus Environment

The Journal of Physical Chemistry

Most related studies in the literature deal with square systems, with uniform stick length and

uniformly distributed angular anisotropy,2,16,24 but the issue of anisotropy has also attracted a great

deal of attention in recent years. Du, Fischer, and Winey10 studied the effect of the alignment of

carbon nanotubes on the percolation in their polymer/nanotube composites. Their experiments and

simulations introduce the interesting point that angular dispersion also can produce (besides stick

density) a percolation transition with critical behavior. Our work is different from or goes beyond

theirs in a number of ways. Importantly, we concentrate on TEA, monitored via the percolation

probability in only one direction in rectangular systems. Furthermore, we gave the sticks realistic

log-normal distributions for their lengths and Gaussian distributions for their azimuthal angles, and

considered rectangular samples. These conditions were dictated by our own experimental MRE

samples. Instead, Du et al.10 considered in their simulations monodispersed (fixed length) sticks,

their angular dispersion is uniform within an angle interval (a wedge"), and they focused on square

systems. More recently, Zheng et al.25 reported on numerical simulations of three-dimensional

percolation of cylindrical rods with both isotropic and anisotropic angular distributions. They

study the effect of the aspect ratio of the percolating objects, and consider monodisperse (identical)

rods. For anisotropic systems they consider a particular type of angular distribution produced by

the interaction with a flow. White et al.26 consider the issue of alignment in percolation of soft-

core cylindrical particles, employing a continuous angular distribution, as a function of which they

study the percolation transition in 3D square systems. Besides the 3D nature of the system and

the different choice of angular distribution, a major difference with our present study is again the

fact that they do not focus on TEA but rather on general percolation, like it is done also in Ref. [

25]. The horizontal-only percolation transition that we focus on here has recently been considered,

for percolation of sticks, among other objects, by Mertens and Moore.27 (see also Ref. [ 28]).

However, their main goal is to introduce a new simulation technique for continuum percolation

models, and for the case of stick percolation they only compute the wrapping percolation threshold

for square systems with isotropically distributed sticks. In turn, in the present work we study

stick percolation in rectangular systems with log-normal length distributions and Gaussian angular

5

Page 5 of 35

ACS Paragon Plus Environment

The Journal of Physical Chemistry

distributions, and explore the full range of parameters of those two distributions in search of TEA.

As a result of our simulations, we are able to specify the special safety zones" of parameter space

where that goal is achieved.

2 Algorithm of Stick-Percolation Simulations

We study two-dimensional stick percolation by means of computer simulations. The percolation

probabilities are obtained by repeating a large number of times a percolation experiment (a real-

ization). Each experiment consists of, starting with an empty rectangular (sides Lx,Ly, aspect ratio

r = Lx/Ly) or square (side L= Lx = Ly) box, adding a desired number N of sticks of length ` (either

a fixed length or statistically distributed values), and determining whether a spanning cluster exists

between the vertical and/or horizontal faces of the box. The orientation of a stick is given by an

angle with respect to a horizontal axis, also generated randomly, with in general .

Depending on the characteristics of the physical system that one wishes to simulate, different sta-

tistical distributions for the lengths ` and the angles can be adopted. For example, the simplest

and most usually studied model is the one with a uniform length for all sticks and...

Recommended